Author
tspani
View
891
Download
4
Embed Size (px)
Natti Rao / Keith O'Brien
Design Data for Plastics Engineers
Hanser Publishers, Munich Hanser/Gardner Publications, Inc., Cincinnati
The Authors: Dr.Ing. NattiRao, Schieferkopf 6,67434 Neustadt, Germany; Dr. Keith T. O'Brien, Vistakon, Ing., 4500 Salisbury Road, Jacksonville, FL 322160995, USA
Distributed in the USA and in Canada by Hanser/Gardner Publications, Inc. 6915 Valley Avenue, Cincinnati, Ohio 452443029, USA Fax: (5B) 5278950 Phone: (5B) 5278977 or 18009508977 Internet: http: //www.hansergardner.com Distributed in all other countries by CarlHanserVerlag Postfach 86 04 20,81631 Munchen, Germany Fax:+49 (89) 9812 64 The use of general descriptive names, trademarks, etc., in this publication, even if the former are not especially identified, is not to be taken as a sign that such names, as understood by the Trade Marks and Merchandise Marks Act, may accordingly be used freely by anyone. While the advice and information in this book are believed to be true and accurate at the date of going to press, neither the authors nor the editors nor the publisher can accept any legal responsibility for any errors or omissions that may be made. The publisher makes no warranty, express or implied, with respect to the material contained herein.
Library of Congress CataloginginPublication Data Rao,NattiS. Design data for plastics engineers / Natti Rao, Keith O'Brien. p. cm. Includes bibliographical references and index. ISBN l56990264X(softcover) 1. Plastics. I. O'Brien, Keith, T. II. Title. TP1120.R325 1998 668.4dc21 9837253
Die Deutsche Bibliothek  CIPEinheitsaufnahme Rao, Natti S.: Design data for plastics engineers / Natti Rao/Keith O'Brien. Munich: Hanser; Cincinnati: Hanser/Gardner, 1998 ISBN 3446210105
All rights reserved. No part of this book may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopying or by any information storage and retrieval system, without permission in writing from the publisher. Carl Hanser Verlag, Munich 1998 Cameraready copy prepared by the authors. Printed and bound in Germany by Druckhaus "Thomas Muntzer", Bad Langensalza
PrefaceMechanical, thermal and rheological properties of polymers form the basic group of property values required for designing polymer machinery. In addition, knowledge of the properties of the resin such as stock temperature of the melt is necessary for optimizing the process. Furthermore, while designing a plastic part, performance properties of the resin depending on the application are to be considered, examples of which are flammability, weather resistance and optical properties, to quote a few. Hence, a variety of property values is needed to accomplish machine design, part design and process optimization. Comprehensive as well as specific overviews of polymer property data exist in the literature. Also the data banks of resin manufacturers offer quick information on thermophysical properties of polymers. But there are few books dealing with both resin and machine design data based on modern findings. The intent of this book is first of all to create an easy to use quick reference work covering basic design data on resin, machine, part and process, and secondly, to show as to how this data can be applied to solve practical problems. With this aim in mind numerous examples are given to illustrate the use of this data. The calculations involved in these examples can be easily handled with the help of handheld calculators. Chapters 1 to 5 deal with the description of physical properties  mechanical, thermal, rheological, electrical and optical  of polymers and principles of their measurement. In Chapter 6 the effect of external influences on the performance of polymers is treated. General property data for different materials such as liquid crystal polymers, structural foams, thermosetting resins and reinforced plastics are given at the end of this chapter. In Chapter 7 the processing properties and machine related data are presented for continuous extrusion processes namely blown film, pipe and flat film extrusion. Resin and machine parameters for thermoforming and compounding have also been included in this chapter. Chapter 8 deals with blow molding and the influence of resin and machine variables on different kinds of blow molding processes. Finally, Chapter 9 covers resindependent and machine related parameters concerning the injection molding process. Machine element design covered in Chapters 7 to 9 includes screw design for extruders and injection molding machines, die design for extruders, mold design for
molding and forming operations and downstream equipment for extrusion. Wherever appropriate, the properties and machine related parameters are described by mathematical formulas which are, as already mentioned, illustrated by workedout examples. The solution procedure used in these examples describes the application of polymer data to solve practical problems. On the basis of this approach the importance of polymer data in dealing with design and process optimization is explained. This book is intended for beginners as well as for practicing engineers, students and teachers in the field of plastics technology and also for scientists from other fields who deal with polymer engineering. We wish to express our sincere thanks to Professor Stephen Orroth of the University of Massachusetts at Lowell, U.S.A., for his valuable suggestions, criticism and review of the manuscript. He also suggested to write a book on the lines of Glanvill's Plastics Engineer's Data Book. Our work is based on the findings of modern plastics technology, and can be considered as an extension to Glanvill's book. The authors also wish to express particular thanks to Dr. Giinter Schumacher of University of Karlsruhe, Germany, for his constructive comments and his great help in preparing the manuscript.
Neustadt, Germany Jacksonville, U.S.A.
Natti S. Rao, Ph.D. Keith T. O'Brien, Ph.D.
AFINALWORD There are many other processes in wide application such as reaction injection molding, compression and transfer molding used to produce parts from thermosetting resins. It was not possible to cover all these processes within the scope of this book. However, the nature of data needed for designing machinery for these processes is similar to the one presented in this work.
Authors Natti S. Rao obtained his B.Tech(Hons) in Mechanical Engineering and M.Tech in Chemical Engineering from the Indian Institute of Technology, Kharagpur, India. After receiving his Ph.D. from the University of Karlsruhe, Germany he worked for the BASF AG for a number of years. Later on he served as a technical advisor to the leading German Plastics machine manufacturers. Natti has published over 50 papers on different aspects of plastics engeneering and authored 3 books on designing polymer machinery with computers. Prior to starting his consultancy company in 1987, he worked as a visiting professor at the Indian Institute of Technology, Chennai(Madras), India. Besides consultancy work, he also holds seminars teaching the application of his software for designing extrusion and injection molding machinery. Keith O'Brien has a B.Sc.(Eng) from the University of London, and M. Sc. and Ph.D. degrees from the University of Leeds in Mechanical Engineering. Keith has over 100 published works to his credit, and also edited the wellknown book, 1 Computer Modeling for Extrusion and other Continuous Processes'. Before he joined Johnson & Johnson, he was professor of mechanical engineering at the New Jersey Institute of Technology.
Contents
Preface .................................................................................... A Final Word ............................................................................ Authors .................................................................................... 1. Mechanical Properties of Solid Polymers ......................1.1 Ideal Solids .............................................................................. 1.2 Tensile Properties ................................................................... 1.2.1 StressStrain Behavior ............................................ 1.2.2 Tensile Modulus ...................................................... 1.2.3 Effect of Temperature on Tensile Strength .............. 1.3 Shear Properties ..................................................................... 1.3.1 Shear Modulus ........................................................ 1.3.2 Effect of Temperature on Shear Modulus ................ 1.4 Compressive Properties .......................................................... 1.4.1 Bulk Modulus .......................................................... 1.5 Time Related Properties ......................................................... 1.5.1 Creep Modulus ....................................................... 1.5.2 Creep Rupture ........................................................ 1.5.3 Relaxation Modulus ................................................ 1.5.4 Fatigue Limit ...........................................................
v vii viii 11 1 2 5 6 6 6 7 9 10 11 11 12 13 14
This page has been reformatted by Knovel to provide easier navigation.
vii
viii
Contents1.6 Hardness ................................................................................. 1.7 Impact Strength ....................................................................... 1.8 Coefficient of Friction .............................................................. 15 17 17
2. Thermal Properties of Solid and Molten Polymers .......2.1 Specific Volume ....................................................................... 2.2 Specific Heat ........................................................................... 2.3 Thermal Expansion Coefficient ............................................... 2.4 Enthalpy ................................................................................... 2.5 Thermal Conductivity .............................................................. 2.6 Thermal Diffusivity ................................................................... 2.7 Coefficient of Heat Penetration ............................................... 2.8 Heat Deflection Temperature .................................................. 2.9 Vicat Softening Point ............................................................... 2.10 Flammability ............................................................................
2323 26 27 29 29 31 32 34 35 35
3. Transport Properties of Molten Polymers ......................3.1 Newtonian and NonNewtonian Fluids ................................... 3.2 Viscous Shear Flow ................................................................ 3.2.1 Apparent Shear Rate .............................................. 3.2.2 Entrance Loss ......................................................... 3.2.3 True Shear Stress ................................................... 3.2.4 Apparent Viscosity .................................................. 3.2.5 True Shear Rate ..................................................... 3.2.6 True Viscosity ......................................................... 3.3 Rheological Models ................................................................. 3.3.1 Hyperbolic Function of Prandtl and Eyring .............. 3.3.2 Power Law of Ostwald and De Waele ..................... 3.3.3 Polynomial of Muenstedt .........................................
3939 41 41 42 42 44 47 47 47 48 48 50
This page has been reformatted by Knovel to provide easier navigation.
Contents3.3.4 Viscosity Equation of Carreau ................................. 3.3.5 Viscosity Formula of Klein ....................................... 3.4 Effect of Pressure on Viscosity ............................................... 3.5 Dependence of Viscosity on Molecular Weight ...................... 3.6 Viscosity of TwoComponent Mixtures ................................... 3.7 Melt Flow Index ....................................................................... 3.8 Tensile Viscosity ...................................................................... 3.9 Viscoelastic Properties ............................................................ 3.9.1 Primary Normal Stress Coefficient ....................... 3.9.2 Shear Compliance Je .............................................. 3.9.3 Die Swell .................................................................
ix53 55 56 57 59 59 60 60 61 61 62
4. Electrical Properties ........................................................4.1 Surface Resistivity ................................................................... 4.2 Volume Resistivity ................................................................... 4.3 Dielectric Strength ................................................................... 4.4 Relative Permittivity ................................................................. 4.5 Dielectric Dissipation Factor or Loss Tangent ........................ 4.6 Comparative Tracking Index (CTI) ..........................................
6565 65 65 66 66 68
5. Optical Properties of Solid Polymers .............................5.1 Light Transmission .................................................................. 5.2 Haze ........................................................................................ 5.3 Refractive Index ...................................................................... 5.4 Gloss ....................................................................................... 5.5 Color ........................................................................................
7373 73 73 75 75
6. External Influences ..........................................................6.1 Physical Interactions ............................................................... 6.1.1 Solubility .................................................................This page has been reformatted by Knovel to provide easier navigation.
7777 77
x
Contents6.1.2 Environmental Stress Cracking (ESC) .................... 6.1.3 Permeability ............................................................ 6.1.4 Absorption and Desorption ...................................... 6.1.5 Weathering Resistance ........................................... 6.2 Chemical Resistance .............................................................. 6.2.1 Chemical and Wear Resistance to Polymers .......... 6.3 General Property Data ............................................................ 77 79 80 80 81 81 82
7. Extrusion ..........................................................................7.1 Extrusion Screws .................................................................... 7.2 Processing Parameters ........................................................... 7.2.1 ResinDependent Parameters ................................. 7.2.2 Machine Related Parameters ..................................
9192 92 92 98
7.3 Extrusion Dies ......................................................................... 124 7.3.1 Pipe Extrusion ......................................................... 126 7.3.2 Blown Film .............................................................. 135 7.3.3 Sheet Extrusion ...................................................... 137 7.4 Thermoforming ........................................................................ 142 7.5 Compounding .......................................................................... 146 7.6 Extrudate Cooling .................................................................... 149 7.6.1 Dimensionless Groups ............................................ 152
8. Blow Molding .................................................................... 1558.1 Processes ................................................................................ 155 8.1.1 Resin Dependent Parameters ................................. 155 8.1.2 Machine Related Parameters .................................. 161
9. Injection Molding .............................................................. 1699.1 ResinDependent Parameters ................................................ 170 9.1.1 Injection Pressure ................................................... 170This page has been reformatted by Knovel to provide easier navigation.
Contents
xi
9.1.2 Mold Shrinkage and Processing Temperature ........ 172 9.1.3 Drying Temperatures and Times ............................. 174 9.1.4 Flow Characteristics of InjectionMolding Resins ..................................................................... 175 9.2 Machine Related Parameters ................................................. 179 9.2.1 Injection Unit ........................................................... 179 9.2.2 Injection Molding Screw .......................................... 180 9.2.3 Injection Mold .......................................................... 183
Index ....................................................................................... 205
This page has been reformatted by Knovel to provide easier navigation.
1
Mechanical Properties of Solid Polymers
The properties of polymers are required firstly to select a material which enables desired performance of the plastics component under conditions of its application. Furthermore they are also essential in design work to dimension a part from a stress analysis or to predict the performance of a part under different stress situations involved. Knowledge of polymer properties is, as already mentioned in the preface, a prerequisite for designing and optimizing polymer processing machinery. In addition to the physical properties there are certain properties known as performance or engineering properties which correlate with the performance of the polymer under varied type of loading and environmental influences such as impact, fatigue, high and low temperature behavior and chemical resistance. The following sections deal with the physical as well as important performance properties of polymers.
1.1 Ideal SolidsIdeal elastic solids deform according to Hookean law which states that the stress is directly proportional to strain. The behavior of a polymer subjected to shear or tension can be described by comparing its reaction to an external force with that of an elastic solid under load. To characterize ideal solids, it is necessary to define certain quantities as follows [3]:
1.2 Tensile PropertiesThe axial force Fn in Fig. 1.1 causes an elongation A/ of the sample of diameter d0 and length I0 fixed at one end. Following equations apply for this case: Engineering strain: (1.2.1)
Hencky strain: (1.2.2) Tensile stress: (1.2.3) Reference area: (1.2.4) Poisson's ratio: (1.2.5)
Fig. 1.1: Deformation of a Hookean solid by a tensile stress [10]
1.2.1 StressStrain BehaviorAs shown in Fig. 1.2 most metals exhibit a linear stressstrain relationship (curve 1), where as polymers being viscoelastic show a nonlinear behavior (curve 2). When the stress is directly proportional to strain the material is said to obey Hooke's law. The slope of the straight line portion of curve 1 is equal to the modulus of elasticity. The maximum stress point on the curve, up to which stress and strain remain proportional is called the proportional limit (point P in Fig. 1.2) [I].
Stress c
Strain z Fig. 1.2: Typical stressstrain curves of metals and polymers Most materials return to their original size and shape, even if the external load exceeds the proportional limit. The elastic limit represented by the point E in Fig. 1.2 is the maximum load which may be applied without leaving any permanent deformation of the material. If the material is loaded beyond its elastic limit, it does not return to its original size and shape, and is said to have been permanently deformed. On continued loading a point is reached at which the material starts yielding. This point (point Y in Fig. 1.2) is known as the yield point, where an increase in strain occurs without an increase in stress. It should however be noted that some materials may not exhibit a yield point. The point B in Fig. 1.2 represents break of the material.
Stress 6
Strain E Fig. 1.3: Secant modulus [3] Owing to their nonlinear nature it is difficult to locate the straight line portion of the stressstrain curve for polymeric materials (Fig. 1.3). The secant modulus represents the
ratio of stress to strain at any point (S in Fig. 1.3) on the stressstrain diagram and is equal to the slope of the line OS. It is an approximation to a linear response over a narrow, but prespecified and standard level of strain [2], which is usually 0.2%. The initial modulus is a straight line drawn tangent to the initial region of the stressstrain curve to obtain a fictive modulus as shown in Fig. 1.4. As this is ambiguous, the resin manufacturers provide a modulus with the stress, for example, G05 corresponding to a strain 0.5 % to characterize the material behavior on a practical basis (Fig. 1.4) [3], This stress G0 is also known as the proof stress. Nm m2 /
Stress 6
Sr i S tan
%
Fig. 1.4: Stress at a strain of 0.5% [3]
mm2 psi
Tensile stress
Elongation
%
Fig. 1.5: Tensile stress diagram of a number of materials at 23C [ 4 ]: a: steel, b: copper, c: polycarbonate, d: PMMA, e: PEHD, f: rubber, g: PELD, h: PVCP
Tensile stress
Stressstrain diagrams are given in Fig. 1.5 for a number of materials [4]. It can be seen from Fig. 1.5 that the advantage of metals lies in their high strength, where as that of plastics lies in their high elongation at break. 1.2.2 Tensile Modulus According to Eq. (1.2.1) and Eq. (1.2.3) one obtains for the modulus of elasticity E which is known as Young's Modulus E = az/ 8 (1.2.6) The modulus of elasticity in a tension test is given in Table 1.1 for different polymers [7]. Table 1.1: Guide Values of Modulus of Elasticity of Some Plastics [4] Material PELD PEHD PP PVCU PS ABS PC POM PA6 PA66 PMMA PET PBT PSU CA CAB PhenolFormaldehydeResins UreaFormaldehydeResins MelaminFormaldehydeResins Unsaturated Polyester Resins Modulus of elasticity N mm'2 200/500 700/1400 1100/1300 1000/3500 3200/3500 1900/2700 2100/2500 2800/3500 1200/1400 1500/2000 2700/3200 2600/3100 1600/2000 2600/2750 1800/2200 1300/1600 5600/12000 7000/10500 4900/9100 14000/20000
The 3.5 % flexural stresses of thermoplastics obtained on a 3point bending fixture (Fig. 1.6) [6] lie in the range 100 to 150 N mm"2 and those of thermosets from around 60 to 150 N mm"2 [7].
A pi d l a p le o d
Fig. 1.6: Three point bending fixture [6]
1.2.3 Effect of Temperature on Tensile StrengthThe tensile strength is obtained by dividing the maximum load (point M in Fig. 1.2) the specimen under test will withstand by the original area of crosssection of the specimen. Fig. 1.7 shows the temperature dependence of the tensile strength of a number of plastics [4].
1.3 Shear PropertiesFigure 1.8 shows the influence of a shear force Ft acting on the area A of a rectangular sample and causing the displacement AU. The valid expressions are defined by: Shear strain: (1.3.1) Shear stress (1.3.2)
1.3.1 Shear ModulusThe ratio of shear stress to shear strain represents the shear modulus G. From the equations above results: (1.3.3)
N mm2 psi Tensile stress Temperature0
Tensile stress
C
Fig. 1.7: Temperature dependence of the tensile stress of some thermoplastics under uniaxial loading [4]; a: PMMA, b: SAN, c: PS, d: SB, e: PVCU f: ABS, g: CA, h: PEHD, i: PELD, k: PELDV
Fig. 1.8: Deformation of a Hookean solid by shearing stress [10]
1.3.2 Effect of Temperature on Shear ModulusThe viscoelastic properties of polymers over a wide range of temperatures can be better characterized by the complex shear modulus G* which is measured in a torsion pendulum test by subjecting the specimen to an oscillatory deformation Fig. 1.9 [2]. The complex shear modulus G* is given by the expression [2] (1.3.4) The storage modulus G' in Eq. (1.3.4) represents the elastic behavior associated with energy storage and is a function of shear amplitude, strain amplitude and the phase angle
5 between stress and strain. The loss modulus G" which is a component of the complex modulus depicts the viscous behavior of the material and arises due to viscous dissipation.
8 TM (t) IE Fig. 1.9: Torsion pendulum; Loading mode and sinusoidal angular displacement t [2] The tangent of the phase angle 8 is often used to characterize viscoelastic behavior and is known as loss factor. The loss factor d can be obtained from (1.3.5) The modulustemperature relationship is represented schematically in Fig. 1.10 [2], from which the influence of the transition regions described by the glass transition temperature Tg and melting point Tm is evident. This kind of data provides information on the molecular structure of the polymer. The storage modulus G' which is a component of the complex shear modulus G* and the loss factor d are plotted as functions of temperature for high density polyethylene in Fig. 1.11 [4]. These data for various polymers are given in the book [4].
DEFORMATION RESISTANCE
HR AD B I TE RT L SL OI D
8
TUH OG SL OI D
VC U SOS I ML ET
R BE Y UBR
TEMPERATURE Fig. 1.10: Generalized relationship between deformation resistance and temperature for amorphous (solid line) and semicrystalline (broken line) high polymers [2]
psi
N/mm2
Dynamic shear modulus G'
Temperature
C
Fig. 1.11: Temperature dependence of the dynamic shear modulus, G' and the loss factor d, obtained in the torsion pendulum test DIN 53445 [4]: PEHD (highly crystalline), PEHD (crystalline), PELD (less crystalline)
1.4 Compressive PropertiesThe isotropic compression due to the pressure acting on all sides of the parallelepiped shown in Fig. 1.12 is given by the engineering compression ratio K . (1.4.1) where AV is the reduction of volume due to deformation of the body with the original volume F0.P P
V0LV
Fig. 1.12: Hookean solid under compression [44]
Mechanical loss factor d
Table 1.2: Poisson ratio ju, density p, bulk modulus K and specific bulk modulus for some materials [10] Material Poisson ratio ju Density p at 200C g/cm3 7.8. 2.7 8.9 2.65 2.5 1.05 1.17 1.08 0.91 0.92 1 0.9 Bulk modulus K N/m2 1.661011 71010 1.344011 3.91010 3.71010 3109 4.1109 3.3109 0.033109 0.7109 2109 1.33109 Specific bulk modulus KJp m2/s2 2.1107 2.6107 1.5107 1.47107 1.494 O7 2.85407 3.5407 2.3407 0.044 O7 3.7407 24 O6 1.5406
Mild steel Aluminum Copper Quartz Glass Polystyrene Polymethylmethacrylate Polyamide 66 Rubber PELD Water Organic liquids
0.27 0.33 0.25 0.07 0.23 0.33 0.33 0.33 0.49 0.45 0.5 0.5
1.4.1 Bulk ModulusThe bulk modulus K is defined by K =p IK (1.4.2)
where A: is calculated from Eq. (1.4.1). The reduction of volume, for instance for PELD, when the pressure is increased by 100 bar follows from Table AV / V0 = 100/(0.7 104) = 1.43% . Furthermore, the relationship between E, G and K is expressed as [3] E = 2 G(I + JU) = 3K(I 2ju) . (1.4.3) This leads for an incompressible solid (K > oo, /j > 0.5 ) to E = 3G. (1.4.4) Typical values of moduli and Poisson's ratios for some materials are given in Table 1.2 [10]. Although the moduli of polymers compared with those of metals are very low, at equal weights, i.e. ratio of modulus to density, polymers compare favorably.
1.5 Time Related Properties1.5.1 Creep Modulus In addition to stress and temperature, time is an important factor for characterizing the performance of plastics. Under the action of a constant load a polymeric material experiences a time dependent increase in strain called creep. Creep is therefore the result of increasing strain over time under constant load [6]. Creep behavior can be examined by subjecting the material to tensile, compressive or flexural stress and measuring the strain for a range of loads at a given temperature. The creep modulus E c in tension can be calculated from E c (t) = W(t) (1.5.1) and is independent of stress only in the linear elastic region. As shown in Fig. 1.13 the creep data can be represented by creep plots, from which the creep modulus according to Eq. (1.5.1) can be obtained. The time dependence of tensile creep modulus of some thermoplastics at 2O0C is shown in Fig. 1.14 [5]. The 2 % elasticity limits of some thermoplastics under uniaxial stress are given in Fig. 1.15. Creep data measured under various conditions for different polymers are available in [4].
a Strain
Te/ m i b
Stress 6
Stress 6
Tet m i
Strain
Fig. 1.13: Longterm stressstrain behavior [3]
Tensile Creep Modulus GN/m2
Nylon 662 20 MN/m
200P Polyethersulfone 28 MN/nf Polysulfone 28 MN/m2 Polycarbonate 20.6 MN/m2
Data for polysulfooe, polycarbonate, Acetal copolymer acretal copolymer and nylon 66 20 MN/m2 from Modern Plastics Encyclopaedia 1 We ek 1 Ya er Time (hours)
Fig. 1.14: Tensile creep modulus vs time for engineering thermoplastics [5] N mm2 psi
Tensile stress
h Stress duration Fig. 1.15:2% elasticity limits of some thermoplastics under uniaxial stress at 200C [4] a: SAN, b: ABS, c: SB, d: chlorinated polyether, e: PEHD, f: PELD
1.5.2 Creep RuptureFailure with creep can occur when a component exceeds an allowable deformation or when it fractures or ruptures [6]. Creep rupture curves are obtained in the same manner as creep, except that the magnitude of the stresses used is higher and the time is measured up
Tensile stress
to failure. Data on creep rupture for a number of polymers are presented in [4]. According to [4] the extrapolation of creep data should not exceed one unit of logarithmic time and a strain elongation limit of 20 % of the ultimate strength. 1.5.3 Relaxation Modulus The relaxation behavior of a polymer is shown in Fig. 1.16 [3]. Relaxation is the stress reduction which occurs in a polymer when it is subjected to a constant strain. This data is of significance in the design of parts which are to undergo longterm deformation. The relaxation modulus of PEHDHMW as a function of stress duration is given in Fig. 1.17 [4]. Similar plots for different materials are to be found in [4].
t>t
r
7
tFig. 1.16: Relaxation after step shear strain y0 [3]
psi
N/mm2Relaxation modulus
Stress duration
h
Fig. 1.17: Relaxation modulus of PEHDHMW as a function of stress duration at 23C [4]
1.5.4 Fatigue LimitFatigue is a failure mechanism which results when the material is stressed repeatedly or when it is subjected to a cyclic load. Examples of fatigue situations are components subjected to vibration or repeated impacts. Cyclic loading can cause mechanical deterioration and fracture propagation resulting in ultimate failure of the material. Fatigue is usually measured under conditions of bending where the specimen is subjected to constant deflection at constant frequency until failure occurs. The asymptotic value of stress shown in the schematic fatigue curve (SN plot) in Figs. 1.18 and 1.19 [6] is known as the fatigue limit. At stresses or strains which are less than this value failure does not occur normally.
SN cuive 
Stress
Log cycles
Fig. 1.18: Fatigue curve [6]
Stress
Fatigue limit
Log cycles (to failure)
Fig. 1.19: Fatigue limit [6]
Some materials do not exhibit an asymptotic fatigue limit. In these cases, the endurance limit which gives stress or strain at failure at a certain number of cycles is used (Fig. 1.20) [6].
Stress
Endurance limitLog cycles (to failure)
Fig. 1.20: Endurance limit [6] For most plastics the fatigue limit is about 20 to 30 % of the ultimate strength measured in shortterm tensile investigations [6]. The Woehler plots for oscillating flexural stress for some thermoplastics are given in Fig. 1.21. Fatigue limits decrease with increasing temperature, increasing frequency and stress concentrations in the part [4].
1.6 HardnessVarious methods of measuring the hardness of plastics are in use. Their common feature is measuring the deformation in terms of the depth of penetration which follows indentation by a hemisphere, cone or pyramid depending on the test procedure under defined load conditions. According to the type of indenter (Fig. 1.22) used the Shore hardness, for example, is given as Shore A or Shore D, Shore A data referring to soft plastics and Shore D to hard plastics. The results of both methods are expressed on a scale between 0 (very soft plastics) and 100 (very hard surface). The ballindentation hardness which represents the indentation depth of a spherical steel indenture is given in Table 1.3 for some thermoplastics [2].
N mm2 psi
Stress amplitude
Cycles to failure Fig. 1.21: Flexural fatigue strength of some thermoplastics [4] a: acetal polymer, b: PP, c: PEHD, d: PVCU Table 1.3: BallIndentation Hardness for Some Plastics [7] Material PELD PEHD PP PVCU PS ABS PC POM PA6 PA66 PMMA PET PBT PhenolFormaldehydeResins UreaFormaldehydeResins MelaminFormaldehydeResins Unsaturated Polyester Resins Hardness N/mm2 13/20 40/65 36/70 75/155 120/130 80/120 90/110 150/170 70/75 90/100 180/200 180/200 150/180 250 320 260/350 260/410 200/240
a;
b)
Fig. 1.22: Types of indenter [7] a: shore, b: shore C and A
1.7 Impact StrengthImpact strength is the ability of the material to withstand a sudden impact blow as in a pendulum test, and indicates the toughness of the material at high rates of deformation. The test procedures are varied. In the Charpy impact test (Fig. 1.23) [2] the pendulum strikes the specimen centrally leading to fracture.
rd s ai u r
Fig. 1.23: Charpy impact test [2]
1.8 Coefficient of FrictionAlthough there is no consistent relationship between friction and wear, the factors affecting the two processes such as roughness of the surfaces, relative velocities of the parts in contact and area under pressure are often the same. Table 1.4 shows the coefficients of sliding friction and sliding wear against steel for different materials [4]. In applications where low friction and high wear resistance are required, smooth surface and low coefficient of friction of the resin components involved are to be recommended.
A typical impact curve as a function of temperature is shown in Fig. 1.24 [6]. This type of data provides the designer with information about the temperature at which the ductile fracture changes to brittle fracture thus enabling to evaluate the performance of the material in a given application. The results of impact tests depend on the manufacturing conditions of the specimen, notch geometry and on the test method. Impact strengths for various plastics are given by Domininghaus [4]. Charpy notched impact strengths of some plastics as functions of notch radius are given in Fig. 1.25 [5].
Impact value
Ductile behaviour Ductile/brittle transition Brittle behaviour
Temperature
Fig. 1.24: Impact curve [6]
PC V Charpy Impact Strength (kj/m2)
Polyethersulfone Nylon 66 (dry)
Acetal AS B Glassfiled nylon Acrylic
Radius (mm)Fig. 1.25: Charpy impact strength vs. notch radius for some engineering thermoplastics [5]
Table 1.4: Coefficient of Sliding Friction of Polymer/Case Hardened Steel after 5 or 24 Hours [4] Polymer Polyamide 66 Polyamide 6 Polyamide 6 {in situ polymer) Polyamide 610 Polyamide 11 Polyethyleneterephthalate Acetal homopolymer Acetal copolymer Polypropylene PEHD (high molecular weight) PEHD (low molecular weight) PELD Polytetrafluoroethylene PA 66 + 8% PELD Polyacetal + PTFE PA 66 + 3% MoS2 PA 66  GF 35 PA 6  GF 35 Standard polystyrene Styrene/Acrylonitrile copolymer Polymethylmethacrylate Polyphenylene ether Coefficient of sliding friction 0.25/0.42 0.38/0.45 0.36/0.43 0.36/0.44 0.32/0.38 0.54 0.34 0.32 0.30 0.29 0.25 0.58 0.22 0.19 0.21 0.32/0.35 0.32/0.36 0.30/0.35 0.46 0.52 0.54 0.35 Sliding frictional wear 0.09 0.23 0.10 0.32 0.8 0.5 4.5 8.9 11.0 1.0 4.6 7.4 21.0 0.10 0.16 0.7 0.16 0.28 11.5 23 4.8 90
Example [8]: The following example illustrates the use of physical and performance properties of polymers in dealing with design problems. The minimum depth of the simple beam of SAN shown in Fig. 1.26 is to be determined for the following conditions: The beam should support a midspan load of 11.13 N for 5 years without fracture and without causing a deflection of greater than 2.54 mm. Solution: The maximum stress is given by (1.8.1)
where F = load (N) l,h,d = dimensions in (mm) as shown in Fig. 1.26. The creep modulus Ec is calculated from (1.8.2) where f is deflection in mm. The maximum stress from Fig. 1.27 at a period of 5 years (= 43800 h) is crmax = 23.44 N/mm2. Working stress crw with an assumed safety factor S = 0.5: ow = 23.440.5 = 11.72 NJmm1 . Creep modulus Ec a t cr < crw ^ d a period of 5 years from Fig. 1.27: Ec = 2413 NI mm2. Creep modulus with a safety factor S = 0.75: Ec = 24130.75 = 1809.75 NJmm2 . The depth of the beam results from Eq. (1.8.1)
The deflection is calculated from Eq. (1.8.2)
Under these assumptions the calculated/is less than the allowable value of 2.54 mm. This example shows why creep data are required in design calculations and how they can be applied to solve design problems.
Fig. 1.26: Beam under midspan load [8]
mm2
Initial applied stress
h Tm at rupture i e Fig. 1.27: Creep curve of SAN [8]
N mm2
Creep modulus
Time t Fig. 1.28: Creep modulus of SAN [8]
h
Literature 1. 2. 3. 4. 5. 6. 7. Nat, D.S.: A Text Book of Materials and Metallurgy, Katson Publishing House, Ludhiana, India 1980 Birley, A. W.: Haworth, B.: Bachelor, T.: Physics of Plastics, Hanser, Munich 1991 Rao, NS.: Design Formulas for Plastics Engineers, Hanser, Munich, 1991 Domininghaus, K: Plastics for Engineers, Hanser, Munich 1993 Rigby, R.B.: Polyethersulfone in Engineering Thermoplastics: Properties and Applications. Ed.: James M. Margolis. Marcel Dekker, Basel 1985 General Electric Plastics Brochure: Engineering Materials Design Guide Schmiedel, K: Handbuch der Kunststoffpriifung (Ed.), Hanser, Munich 1992
8. Design Guide, Modem Plastics Encyclopedia, 197879 9. Brochure: Advanced CAE Technology Inc. 1992 10. Pahl, M.; Gleifile, W.; Laun, KM.: Praktische Rheologie der Kunststoffe und Elastomere, VDIKunststofftechnik, Dusseldorf 1995
2
Thermal Properties of Solid and Molten Polymers
In addition to the mechanical and melt flow properties thermodynamic data of polymers are necessary for optimizing various heating and cooling processes which occur in plastics processing operations. In design work the thermal properties are often required as functions of temperature and pressure [2]. As the measured data cannot always be predicted by physical relationships accurately enough, regression equations are used to fit the data for use in design calculations.
2.1 Specific VolumeThe volumetemperature relationship as a function of pressure is shown for a semicrystalline PEHD in Fig. 2.1 [1] and for an amorphous PS in Fig. 2.2 [I]. The pvT diagrams are needed in many applications, for example to estimate the shrinkage of plastics parts in injection molding [19]. Data on pvT relationships for a number of polymers are presented in the handbook [8]. According to SpencerGilmore equation which is similar to the VanderWaal equation of state for real gases the relationship between pressure p, specific volume v and temperature T of a polymer can be written as (2.1.1) In this equation b* is the specific individual volume of the macromolecule, p*, the cohesion pressure, W, the molecular weight of the monomer and R, the universal gas constant [9]. The values p* and b* can be determined from pVT diagrams by means of regression analysis. Spencer and Gilmore and other workers evaluated these constants from measurements for the polymers listed in Table 2.1 [9], [18].
S E I I V L M (cm3/g) P CFC OU E
TEMPERATURE(0C)
Fig. 2.1: Specific volume vs. temperature for a semicrystalline polymer (PP) [1]
Specific volume (cm3/g)
Temperature (0C) Fig. 2.2: Specific volume vs. temperature for an amorphous polymer (PS) [1]
Table 2.1: Constants for the Equation of State [9] Material PELD PP PS PC PA 610 PMMA PET PBT W g/mol 28.1 41.0 104 56.1 111 100 37.0 113.2 b* cmVg 0.875 0.620 0.822 0.669 0.9064 0.822 0.574 0.712
atm 3240 1600 1840 3135 10768 1840 4275 2239
Example: Following values are given for a PELD: W b* p* = = = 28.1 g/Mol 0.875 cm7g 3240 arm
Calculate the specific volume at T = 190Candplbar Solution: Using Eq. (2.1.1) and the conversion factors to obtain the volume v in crnVg, we obtain 10 8.314.(273, 190) + y = = 28.13240.991.013 The density p is the reciprocal value of specific volume so that 1 P = v The pvT data can also be fitted by a polynomial of the form v = A(0) v + A(l) v p+ A(2) v T+ A ( 3 ) v T p (2.1.2) if measured data is available (Fig. 2.3) [10], [11], [17]. The empirical coefficients A(0)v... A(3)v can be determined by means of the computer program given in [H]. With the modified twodomain Tait equation [16] a very accurate fit can be obtained both for the solid and melt regions.
cm3/g
/> = 1bar
OO a J br Specific volume v 800 bar
m a ue esrd polynomial0
C
Temperature TFig. 2.3: Specific volume as a function of temperature and pressure for PELD [2], [13]
2.2 Specific HeatThe specific heat cp is defined as (Si),
where h = enthalpy T = Temperature The specific heat cp gives the amount of heat which is supplied to a system in a reversible process at a constant pressure in order to increase the temperature of the substance by dT. The specific heat at constant volume cv is given by
C  [^lwhere u = internal energy T = Temperature In the case of cv the supply of heat to the system occurs at constant volume. cp and cv are related to each other through the SpencerGilmore equation Eq. (2.1.1)
(2.2.3)The numerical values of cp and cv differ by roughly 10 %, so that for approximate calculations cv can be made equal to cp. Plots of cp as function of temperature are shown in Fig. 2.4 for amorphous, semicrystalline and crystalline polymers.
a )
b )
c)
Fig. 2.4: Specific heat as a function of temperature for amorphous (a), semicrystalline (b) and crystalline polymers (c) [14]
(2.2.4)
JiL k K g m aue esrd Specific heat cp pyo a on m l l i
As shown in Fig. 2.5 measured values can be fitted by a polynomial of the type [11]
T m ea r T e prt e u
'C
(2.3.1) The expansion coefficient aY a* constant pressure is pgivenand polynomial for PELD [2] 2.3 Fig. 2.5: Comparison between measured values of c [13] by [14] Thermal Expansion Coefficient
The isothermal compression coefficient yk is defined as [14]
r,   1 [)v \dpJTay and yk are related to each other by the expression [14]Cp Cv + ^ ^
(23.2)(2.3.3)
The linear expansion coefficient alin is approximatelytflin = CCv (2.3.4)
Table 2.2 shows the linear expansion coefficients of some polymers at 20 0C. The linear expansion coefficient of mild steel lies around 11 x 10"6 [K"1] and that of aluminum about 25 x 10~6 [K"1]. As can be seen from Table 2.2 plastics expand about 3 to 20 times more than metals. Factors affecting thermal expansion are crystallinity, crosslinking and fillers
Table 2.2: Coefficients of Linear Thermal Expansion [1], [5] Polymer PELD PEHD PP PVCU PVCP PS ABS PMMA POM PSU PC PET PBT PA 6 PA 66 PTFE TPU Coefficient of linear expansionat 20 0C alin 106K1 250 200 150 75 180 70 90 70 100 50 65 65 70 80 80 100 150
2.4 EnthalpyEq. (2.2.1) leads to dh = cp dT
(2.4.1)
As shown in Fig. 2.6 the measured data on h = h(T) [13] for a polymer melt can be fitted by the polynomial (2.4.2)
kg
p l n ma oy o i l
m a ue esrd
hhn
0
T m eaue T e prtr
C
Fig. 2.6: Comparison between measured values of h [13] and polynomial for PA6 [11] The specific enthalpy defined as the total energy supplied to the polymer divided by the throughput of the polymer is a useful parameter for designing extrusion and injection molding equipment such as screws. It gives the theoretical amount of energy required to bring the solid polymer to the process temperature. Values of this parameter for different polymers are given in Fig. 2.7 [14]. If, for example, the throughput of an extruder is 100 kg/h of polyamide (PA) and the processing temperature is 260 C, the theoretical power requirement would be 20 kW. This can be assumed to be a safe design value for the motor horse power, although theoretically it includes the power supply to the polymer by the heater bands of the extruder as well.
2.5 Thermal ConductivityThe thermal conductivity X is defined as (2.5.1)
kWh kg P P A S P C
Enthalpy
^C V
9
T m ea r I e prt e u
C
Fig. 2.7: Specific enthalpy as a function of temperature [14] where Q = heat flow through the surface of area A in a period of time t (T1T2) = temperature difference over the length 1. Analogous to the specific heat cp and enthalpy h the thermal conductivity X as shown in Fig. 2.8 can be expressed as [2] (2.5.2)
Thermal conductivity A
measured
m K
polynomial
0
C
T m eaue Je prtr Fig. 2.8: Comparison between measured values of A, [13] and polynomial for PP [2]
The thermal conductivity increases only slightly with the pressure. A pressure increase from 1 bar to 250 bar leads only to an increase of less than 5 % of its value at 1 bar.
As in the case of other thermal properties the thermal conductivity is, in addition to its dependence on temperature, strongly influenced by the crystallinity and orientation and by the amount and type of filler in the polymer [I]. Foamed plastics have, for example, thermal conductivities at least an order of magnitude less than those of solid polymers [I].
2.6 Thermal DiffusivityThermal diffusivity a is defined as the ratio of thermal conductivity to the heat capacity per unit volume [1] a = ^P 'Cp
(2.6.1)
and is of importance in dealing with transient heat transfer phenomena such as cooling of melt in an injection mold [2]. Although for approximate calculations average values of thermal diffusivity can be used, more accurate computations require functions of Z, p and cp against temperature for the solid as well as melt regions of the polymer. Thermal diffusivities of some polymers at 20 0C are listed in Table 2.3 [14], [15]. Table 2.3: Thermal Diffusivities of Polymers at 20 0C Polymer PELD PEHD PP PVCU PVCP PS PMMA POM ABS PC PBT PA 6 PA 66 PET I Thermal diffusivity at 20 0C a 106m2/s 012 0.22 0.14 0.12 0.14 0.12 0.12 0.16 0.15 0.13 0.12 0.14 0.12 0.11
Exhaustive measured data of the quantities cp, h, X and pvT diagrams of polymers are given in the VDMAHandbook [8]. Approximate values of thermal properties of use to plastics engineers are summarized in Table 2.4 [14], [15]. Experimental techniques of measuring enthalpy, specific heat, melting point and glass transition temperature by differential thermal analysis (DTA) such as differential scanning calorimetry (DSC) are described in detail in the brochure [12]. Methods of determining thermal conductivity, pvT values and other thermal properties of plastics have been treated in this brochure [12]. Table 2.4: Approximate Values for Thermal Properties of Some Polymers [14] Polymer Thermal conductivity (20 0C) X W/mK 0.12 0.16 0.20 0.12 0.25 0.15 0.23 0.32 0.40 0.49 0.15 0.36 0.37 0.29 0.21 Specific heat (20C)cp kJ/kgK 1.20 1.10 1.45 1.40 1.46 1.40 1.17 2.30 2.30 2.25 2.40 1.70 1.80 1.55 1.25 Density (20 0C) p g/cm3 1.06 1.40 1.18 1.08 1.42 1.02 1.20 0.92 0.92 0.95 0.91 1.13 1.14 1.35 1.35 Glass transition temperature Tg C 101 80 105 115 73 115 150 120/90 120/90 120/90 10 50 55 70 450
Melting point range Tm0
C
PS PVC PMMA SAN POM ABS PC PELD PELLD PEHD PP PA6 PA 66 PET PBT
ca. 175
ca. 110 ca. 125 ca. 130 160/170 215/225 250/260 250/260 ca. 220
2.7 Coefficient of Heat PenetrationThe coefficient of heat penetration is used in calculating the contact temperature which results when two bodies of different temperature are brought into contact with each other [2], [16]. As shown in Table 2.5 the coefficients of heat penetration of metals are much higher than those of polymer melts. Owing to this the contact temperature of the wall of an injection mold at the time of injection lies in the vicinity of the mold wall temperature before injection.
The contact temperature #Wmax of the wall of an injection mold at the time of injection is [17]0W
~
_ bw flWmin + b p Bu " bw + bp
n {JA)
where b = coefficient of heat penetration= J / l p c ^wmjn = temperature before injection 0u = melt temperature Indices w and p refer to mold and polymer respectively. Table 2.5: Coefficients of Heat Penetration of Metals and Plastics [17] Material Beryllium Copper (BeCu25) Unalloyed Steel (C45W3) Chromium Steel (X40Cr 13) Polyethylene (PEHD) Polystyrene (PS) Stainless Steel Aluminum Coefficient of heat penetration b W s05 m'2 K1 17.2 x 103 13.8 x 103 11.7 x 103 0.99 x 103 0.57 x 103 7.56 x 103 21.8 x 103
The values given in Table 2.5 refer to the following units of the properties: Thermal conductivity X: Density p: Specific heat c: The approximate values for steel are 1 = 50 W/(mK) r = 7850 kg/m3 c = 0.485 kJ/(kgK) The coefficient of heat penetration is W/(mK) kg/m3 kJ/(kgK)
2.8 Heat Deflection TemperatureHeat Deflection Temperature (HDT) or the Deflection Temperature under load (DTUL) is a relative measure of the polymer's ability to retain shape at elevated temperatures while supporting a load. In amorphous materials the HDT almost coincides with the glass transition temperature Tg. Crystalline polymers may have lower values of HDT but are dimensionally more stable at elevated temperatures [5]. Additives like fillers have more significant effect on crystalline polymers than on amorphous polymers. The heat deflection temperatures are listed for some materials in Table 2.6. Owing to the similarity of the measuring principle Vicat softening point, HDT and Martens temperature lie often close to each other (Fig. 2.9) [6]. Table 2.6: Heat Deflection Temperatures (HDT) According to the Method A of Measurement [3], [6] Material PELD PEHD PP PVC PS ABS PC POM PA6 PA66 PMMA PET PBT VlCAT load loadstandardized needle heat transfer liquid a) specimen b)
I
HDT (Method A) _C 35 50 45 72 84 100 135 140 77 130 103 80 65 M RE S ATN HT D load
specimen oven c)
heat transfer liquid specimen
Fig. 2.9: Principles of measurement of heat distortion of plastics [6]
2.9 Vicat Softening PointVicat softening point is the temperature at which a small lightly loaded, heated test probe penetrates a given distance into a test specimen [5]. The Vicat softening point gives an indication of the material's ability to withstand contact with a heated object for a short duration. It is used as a guide value for demolding temperature in injection molding. Vicat softening points of crystalline polymers have more significance than amorphous polymers, as the latter tend to creep during the test [5]. Both Vicat and HDT values serve as a basis to judge the resistance of a thermoplastic to distortion at elevated temperatures. Guide values of Vicat softening temperatures of some polymers according to DIN 53460 (Vicat 5 kg) are given in Table 2.7 [6]. Table 2.7: Guide Values for Vicat Softening Points [6] Polymer PEHD PP PVC PS ABS PC POM PA 6 PA 66 PMMA PET Vicat softening point ^C 65 90 92 90 102 138 165 180 200 85 190
PBT
I
180
2.10 FlammabilityMost plastics are flammable and can act as fuel in a fire situation. The aim of various flammability tests is to measure the burning characteristics of plastics materials once ignition has occurred. The Critical Oxygen Index is the most accepted laboratory test. It measures the minimum volume concentration of oxygen in a mixture of oxygen and nitrogen, which is required to initiate combustion of the plastic and propagate flameburning to a prespecified extent (a flamespread time or a distance along the test sample) [I]. Data are presented in the form of Limiting Oxygen Index (LOI) value. These values
are summarized in Table 2.8 [I]. The nonflammability of PTFE is manifested by its exceptionally high LOI value. Other flameresistant plastics include thermosets, PVC and PVDC. Resistance to flammability can be enhanced by adding flame retarding additives to the polymer [I]. Table 2.8: Limiting Oxygen Indices (LOI) of polymers (23 0C) [1] Material POM PMMA PE PP PS ABS PET PA 66 PSU PI PVDC PVC (chlorinated) PTFE I LOI 14.9/15.7 17.4 17.4 17.4 17.6/18.3 18.3/18.8 20.0 24/29 30/32 36.5 60.0 60.0/70.0 95.0
CLAMP PLASTICS SPECIMEN
IGNITION SUC ORE
(V)
(H)
Fig. 2.10: Typical arrangements for the UL flammability test: (V) UL 94 v vertical small flame ignitibility (variable sample thickness); (H) UL 94 HB horizontal small flame ignitibility / flame spread [1]
Underwriters' Laboratory test (UL 94) is a rating system which classifies flammability behavior of plastics according to their ability to maintain combustion after the flame is removed (see Fig. 2.10 [I]). In general, plastics which extinguish rapidly and do not drip flaming particles obtain high ratings. Ratings are given on the basis of minimum wall thickness of the material which corresponds to a particular flame class [I]. These thicknesses are important for designing plastics component design. The temperature index determined on the basis of the tensile halflife concept of the Underwriters' Laboratories is shown for various polymers in Fig. 2.11 [4]. The smoke emission for a number of plastics is given in Fig. 2.12 [4].
Temperature 0C
Fig. 2.11: UL temperature index for some thermoplastics [4]
Specific Optical Density, DM (corr.)
Test Conditions: American National Bureau of Standarts Smoke 32 mm Samples Flamming Condition
Fig. 2.12: Smoke emission behavior of some thermoplastics [4]
Literature 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. Birley, A. W.: Haworth, B.: Bachelor, T.: Physics of Plastics, Hanser, Munich 1991 Rao, N. S.: Design Formulas for Plastics Engineers, Hanser, Munich, 1991 Domininghaus, K: Plastics for Engineers, Hanser, Munich 1993 Rigby, R.B.: Polyethersulfone in Engineering Thermoplastics: Properties and Applications. Ed.: James M. Margolis. Marcel Dekker, Basel 1985 General Electric Plastics Brochure: Engineering Materials Design Guide Schmiedel, K: Handbuch der Kunststoffpriifung (Ed.), Hanser, Munich 1992 Design Guide, Modern Plastics Encyclopedia, 197879 Kenndaten fur die Verarbeitung thermoplastischer Kunststoffe, Teil I, Thermodynamik, Hanser, Munich 1979 Mckelvey, JM.: Polymer Processing, John Wuley, New York 1962 Miinstedt, K: Berechnen von Extrudierwerkzeugen, VDIVerlag, Diisseldorf, 1978 Rao, N.S.: Designing Machines and Dies Polymer Processing, Hanser, Munich 1981 Brochure: Advanced CAE Technology Inc. 1992 Proceedings, 9. Kunststofftechnisches !Colloquium, IKV, Aachen 1978 Rauwendal, C: Polymer Extrusion, Hanser, Munich 1986. Ogorkiewicz, RM.: Thermoplastics Properties and Design, John Wuley, New York 1973 Martin, H.: VDIWarmeatlas, VDIVerlag, Diisseldorf 1984 Wubken, G: Berechnen von SpritzgieBwerkzeugen, VDIVerlag, Diisseldorf 1974 Progelhof, R.C., Throne, J.L.: Polymer Engineering Principles  Properties, Processes, Tests for Design, Hanser, Munich 1993 Kurfess, W.: Kunststoffe 61 (1971), p 421
3
Transport Properties of Molten Polymers
The basic principle of making parts out of polymeric materials lies in creating a melt from the solid material and forcing the melt into a die, the shape of which corresponds to that of the part. Thus, as Fig. 3.1 indicates, melt flow and thermal properties of polymers play an important role in the operations of polymer processing. Plastics solids
Plastication
Melt
Shaping
Cooling
Part removal Fig. 3.1: Principle of manufacturing of plastics parts
3.1 Newtonian and NonNewtonian FluidsAnalogous to the ideal elastic solids there exists a linear relationship between stress and strain in the case of Newtonian fluids (Fig. 3.2).
SHEARSTRESS Dilatant
Bingham Newtonian
Pseudoplastic
SHEAR RATE
Fig. 3.2: Flow curves of idealized fluids [1] The fluid between the upper plate in Fig. 3.3 moving at a constant velocity Ux and the lower stationary plate experiences a shear stress x (see Fig. LIB also). (3.11)
Ux H
Fig. 3.3: Shear flow The shear or deformation rate of the fluid is equal to H dy The shear viscosity is then defined as TJ = (3.1.3)
rFor an extensional flow, which corresponds to the tension test of Hookean solid, we get (3.1.4) where
GZ = normal stress A = Trouton viscosity e = strain rate Analogous to Eq. (1.4.4) one obtains I = 3TJ
(3.1.5)
3.2 Viscous Shear FlowMacromolecular fluids like thermoplastic melts exhibit significant nonNewtonian behavior. This is noticed in the marked decrease of melt viscosity when the melt is subjected to shear or tension as shown in Fig. 3.4 and in Fig. 3.5. The flow of melt in the channels of dies and polymer processing machinery is mainly shear flow. Therefore, knowledge of the laws of shear flow is necessary for designing machines and dies for polymer processing. For practical applications the following summary of the relationships was found to be useful.
3.2.1 Apparent Shear RateThe apparent shear rate for a melt flowing through a capillary is defined as ,  $ where Q is the volume flow rate per second and R, the radius of capillary.
Igq.lg/i M = 31 o
140 120/150 < 150 120/150 < 150 100/120 120/150 120/150 >150 140/175 175/230 100/120 120/150 injection cycle pnri start closing the mold injection unit forward filling
ABS POM PE PA PC PMMA PS Rigid PVC Thermosets Elastomers
opening the mold part ejection
holding pressure plasticating cdounq injection unit backward
Fig. 9. IB: Molding cycle [22]
Injection stageEffects from: injection speed temperature of hydraulic oil. melt and mold viscosity of material pressure dependency of screw drive Effects on o. material: viscosity molecular degradation crystallinity molecular orientation in part surface b. parts: surface quality
Compression stageEffects from* switchover to holding pressure control of pressure reserve Effects on crystallinity anisotropy b. parts: completeness of molded part flash formation weight Time Holding pressure stage Injection stage Compression stage
Holding pressure stageEffects from: temperature of cavity wait deformation of m l od stability of clamping unit magnitude of clamping force Effects on a. material: crystallinity molecular orientatior inside the part shrinkage b. parts: weight dimensions voids sink marks relaxation ease of ejection
Cavity pressure
Fig. 9.1C: Cavity pressure profile over time [1]
9.1.2 Mold Shrinkage and Processing TemperatureDue to their high coefficients of thermal expansion components molded from plastics experience significant shrinkage effects during the cooling phase. Semicrystalline polymers tend to shrink more, owing to the greater specific volume difference between melt and solid. Shrinkage S can be defined by [2] S =1
^
(9.1.1)
where V is any linear dimension of the mold and L, the corresponding dimension of the part when it is at some standard temperature and pressure. As a consequence of mold shrinkage it is necessary to make core and cavity slightly larger in dimension than the size of the finished part. Processing temperature, mold temperature and shrinkage are given in Table 9.2 for a number of materials [I]. The parameters influencing shrinkage behavior are shown in Fig. 9.2 [17].
Table 9.2: Processing Temperatures, Mold Temperatures, and Shrinkage for the Most Common Plastics Processed by Injection Molding [1] MaterialPS HIPS SAN ABS ASA PELD PEHD PP PPGR IB PMP PVCsoft PVCrigid PVDF PTFE FEP PMMA POM PPO PPOGR CA CAB CP PC PCGR PET PETGR PBT PBTGR PA 6 PA 6GR PA 66 PA 66GR PAIl PA 12 PSO PPS PUR PF MF MPF UP EP
Glass fiber content %
Processing temperature 0C180/280 170/260 180/270 210/275 230/260 160/260 260/300 250/270 260/280 150/200 280/310 170/200 180/210 250/270 320/360 210/240 200/210 250/300 280/300 180/230 180/230 180/230 280/320 300/330 260/290 260/290 240/260 250/270 240/260 270/290 260/290 280/310 210/250 210/250 310/390 370 195/230 60/80 70/80 60/80 40/60 ca.70
Mold temperature 0 C10/10 5/75 50/80 50/90 40/90 50/70 30/70 50/75 50/80 70 15/50 30/50 90/100 200/230 50/70 >90 80/100 80/100 50/80 50/80 50/80 80/100 100/120 140 140 60/80 60/80 70/120 70/120 70/120 70/120 40/80 40/80 100/160 > 150 20/40 170/190 150/165 160/180 150/170 150/170
Shrinkage %0.3/0.6 0.5/0.6 0.5/0.7 0.4/0.7 0.4/0.6 1.5/5.0 1.5/3.0 1.0/2.5 0.5/1.2 1.5/3.0 >0.5 0.5 3/6 3.5/6.0 0.1/0.8 1.9/2.3 0.5/0.7 ,
T'
(.,
LNQ^b2T2J
Introducing the given values we get 01 305 104
55 2 I'" = 0.771 2 10 0.174195 U3602;r(0.105) 12j Table 9.7B shows the results of simulating the mold filling of a large rectangular open container (Fig, 9.1 IA) [24] according to the model of Stevenson [12].
Br = f4

{
160 360
'
Fig. 9.1 IA: Mold filling of rectangular open container according to the model of Stevenson [12]
Relative to the standard conditions the results in Table 9.7B show that Ap is decreased by 10 percent when T1 is increased 20 0C, by 4 percent when Tw is increased 20 0C, by 24 percent when the material is changed, by 37 percent when the number of gates is increased to four, and by 63 percent when all of the above changes are made. The optimal conditions which correspond to the lowest Ap and F occur when these changes are combined with the change of the resin.
Table 9.7B: Simulations of Injection Pressure and Clamp Force at Different Processing Conditions [24]
Resin A A A B A B
N
1 1 1 1 4 4
T1 K 501 520 500 500 500 5000
Tw 0 K 301 301 321 301 301 301
Br 1.381 0.962 1.536 0.849 0.625 0.299
Ap MPa 302 273 290 229 192 113
F kN 191000 175000 181000 147000 67800 40400
Symbols in Table 9.7B: T1: inlet melt temperature Tw: mold wall temperature Ap: injection pressure drop F: clamp force N: Number of gates Operating Conditions: injection rate = 2000 crnVs fill time = 3.81 s halfthickness of the part = 0.127 cm dimensionless fill time T = 0.1824 A rough estimate of the clamp force can be made as follows: The pressure drop in a plate mold AP1N for the melt flow of an isothermal, Newtonian fluid can be calculated from Eqns. (7.3.2) and (7.3.4) given in Section 7.3 by putting n = 1. AP1N is then
Substituting the injection rate for the volume flow rate Q 0 we get Q=^ where V = W H L and t = injection time = L/u with u = injection velocity Introducing the equations above into Eq. (9.2.3) we obtain (9.2.4)
APiN=1
ir'r u ' ; 7
(925)
Example with symbols and units in Eq. (9.2.5)
part thickness flow length injection velocity melt viscosity Solution:
H = I mm L = 100 mm u = 100 mm/s r = 250 P s
1O 100 1 100250 OAAU A P l N = 12 ^  = 300bar
In Fig. 9.1 IC AP1N is plotted over the part thickness H for different ratios of flow length L to part thickness H [25]. The injection velocity is assumed to be 10 cm/s and the melt viscosity 250 Pa s. The pressure Apm is then corrected by the following correction factors [26]:Correction Factor CFshape
Depending on the complicacy of the part geometry the factor CFshape can have values between 1.1 to 1.3.Correction Factor CFresin
The correction factors for the flow behavior of the resin CFresin are given in Table 9.7C for some resins. Table 9.7C: Correction Factor CFresin [26] "Resin PE, PP, PS PMMA, PPO PA, SB PC 5 PVC ABS, SAN, CA CFresin 1.0 1.5 1.2 1.7 11.3
Finally the actual cavity pressure Ap Ap = A PlN . CFshape CFresin and the clamp force F [kN] A p(bar) projected area of the part (c m 2 ) 100
[bar]
uncorrected cavity pressure
ratio of flow length to part thickness
part thickness [mm] (a)
[bar] ratio of flow length to part thickness uncorrected cavity pressure
part thickness [mm] (b)Fig. 9.1 IB: Cavity pressure as a function of part thickness and ratio of flow length to part thickness [25]
Example: Diskshaped mold (see Fig. 9.1 IA) Thickness H = I mm Radius R =100 mm Correction factor CFshape =1.2 Resin: ABS CFresin from Table CFresin= 1.3 Solution: Ratio of flow length to part thickness L/H L/H=100 AP1N from Fig. 4.1 IB for L/H = 100 and H = 1 AP1N = 300 bar Actual cavity pressure Ap Ap = 3001.21.3 =468 bar Clamp force F (kN) F = ^ M * 147OkN 100 In Fig. 9.12 the relationship between shot size and clamping force is presented for some commercially available injection molding machines [I]. Here a and a0 are the ratios between working (injection) capacity and clamping force and Fcx and Fco the clamping forces. The following example shows as to how the maximum shot weight can be calculated if the clamping force is known. Example: Clamping force: 3500 kN Value of the ordinate corresponding to the dashed line 3 in Fig. 9.12b: 0.39 Maximum shot weight for polystyrene assuming a density of 0.9: 3500 x 0.39 x 0.9 1230 g Effective maximum shot weight with a factor of 0.8: 1230 x 0.8 980 g The range for the maximum shot weight is approximately [1] 1230 500 g. Twodimensional and threedimensional diagrams as shown in Fig. 9.13 [18] are helpful in the practice for finding out the useful working range of an injection molding machine [18].
Max shot size / clamping force
.cm5 kN
Model lawa=a
_ Max. shot size
3
i d ^ kN
clamping force ^N Clamping force F c cm3 kN Max shot size / clamping force
Model lawa= aa
=
Max. shot size JCUL3 clamping force kN
( F f3 c o 7"^
Clamping force F c
kN
Fig. 9.12: Calculation of maximum shot weight by means of model laws [1]
Ram pressure
F lash area
Molding ' area
Short shot area
Mold temperature
Fig. 9.13: Mold Area Diagram (MAD) and Mold Volume Diagram (MVD) [18] a: MAD, b: MVD
Ram pressure psi
9.2.3.4 Thermal Design of Mold Cooling of Melt in Mold The analytical solution for the transient onedimensional heat conduction for a plate can be written as [13] *  M ^ fe] Although this equation is valid only for amorphous polymers, it has given good results in the practice for semicrystalline and crystalline polymers as well, so that its general use for all thermoplastic materials is justified. Example with symbols and units: Cooling of a part in an injection mold for the following conditions [5]: resin: PELD thickness of the plate s = 12.7 mm temperature of the melt Ta = 243.3 0C = mold temperature Tw 21.10C = demolding temperature Tb 76.7 0C thermal diffusivity of the melt a = 1.2910"3 cm2/s The temperature Tb in Eq. (9.2.6) refers to the centerline temperature of the part. Solution: The temperature ratio 0Th : Q1b = ^ Z J ^ = 7 6  7  2 U =0.25 Tb T 3 Tw 243.321.1 cooling time tk according to Eq. (9.2.6)
tk =
L2?2 2
3  l n f 1 = 206.5 s
The cooling time tk can also be found from Fig. 9.14 in which the ratio 0Th is plotted over the Fourier number for bodies of different geometry [14]. Fourier number F0 from Fig. 9.14 at 0Th = 0.25 F0 = 0.66 Cooling time tk: s 12.7 , . _ x= = = 6.35 mm 2 2
Temperature ratio